Phase Transitions and Structures at 10, 92 and 293 K in Eight Trigonal Double Salts <i>M</i>^I^[<i>M</i>^III^(NH~3~)~6~](ClO~4~)~2~<i>X</i>~2~
Figgis, B. N.; Sobolev, A. N.; Reynolds, P. A.; Acta Crystallographica Section B 54 (1998) 613–625; doi:10.1107/S0108768198002328

data_2003156
_publ_section_title
;
 Phase Transitions and Structures at 10, 92 and 293 K in Eight Trigonal
 Double Salts
 <i>M</i>^I^[<i>M</i>^III^(NH~3~)~6~](ClO~4~)~2~<i>X</i>~2~
;
_journal_issue                   5
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              613
_journal_page_last               625
_journal_paper_doi               10.1107/S0108768198002328
_journal_volume                  54
_journal_year                    1998
_chemical_formula_iupac          'Rb[Ru(N H3)6],2(Cl O4),2Cl'
_chemical_formula_moiety         'Rb1,N6 H18 Ru1,2(ClO4),2Cl'
_chemical_formula_sum            'Cl4 H18 N6 O8 Rb Ru'
_chemical_formula_weight         558.54
_space_group_IT_number           166
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_audit_creation_method           SHELXL
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            3
_cell_length_a                   7.1392(6)
_cell_length_b                   7.1392(6)
_cell_length_c                   27.599(4)
_cell_measurement_reflns_used    18
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      20.17
_cell_measurement_theta_min      16.36
_cell_volume                     1218.2(2)
_computing_cell_refinement       'P3/PC (Siemens, 1989)'
_computing_data_collection       'P3/PC (Siemens, 1989)'
_computing_data_reduction        PROFIT
_computing_publication_material  'SHELXTL (Sheldrick, 1983)'
_computing_structure_refinement  'SHELXL-93 (Sheldrick, 1993)'
_computing_structure_solution    'SHELXS-86 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measurement_device_type  'Siemens P4'
_diffrn_measurement_method       \w/\q
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'normal-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0141
_diffrn_reflns_av_sigmaI/netI    0.0063
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_l_max       38
_diffrn_reflns_limit_l_min       -38
_diffrn_reflns_number            4752
_diffrn_reflns_theta_max         30.01
_diffrn_reflns_theta_min         2.21
_diffrn_standards_decay_%        2
_diffrn_standards_interval_count 100
_diffrn_standards_number         6
_exptl_absorpt_coefficient_mu    4.640
_exptl_absorpt_correction_T_max  0.5515
_exptl_absorpt_correction_T_min  0.3700
_exptl_absorpt_correction_type   gaussian
_exptl_crystal_colour            Yellow
_exptl_crystal_density_diffrn    2.284
_exptl_crystal_description       'Trigonal antiprism'
_exptl_crystal_F_000             819
_exptl_crystal_size_max          0.25
_exptl_crystal_size_mid          0.25
_exptl_crystal_size_min          0.13
_refine_diff_density_max         0.323
_refine_diff_density_min         -0.356
_refine_ls_extinction_coef       0.0046(3)
_refine_ls_extinction_method     'SHELXTL (Sheldrick, 1983)'
_refine_ls_goodness_of_fit_all   1.095
_refine_ls_goodness_of_fit_obs   1.100
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     34
_refine_ls_number_reflns         491
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.095
_refine_ls_restrained_S_obs      1.100
_refine_ls_R_factor_all          0.0151
_refine_ls_R_factor_obs          0.0148
_refine_ls_shift/esd_max         0.01
_refine_ls_shift/esd_mean        0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0263P)^2^+1.0582P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_all         0.0410
_refine_ls_wR_factor_obs         0.0408
_reflns_number_observed          481
_reflns_number_total             491
_reflns_observed_criterion       >2sigma(I)
_cod_data_source_file            ta0002.cif
_cod_data_source_block           V
_cod_depositor_comments
;
The following automatic conversions were performed:
'_exptl_absorpt_correction_type' value 'Gaussian' changed to 'gaussian'
according to '/home/saulius/struct/CIF-dictionaries/cif_core.dic'
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 

The following automatic conversions were performed:

'_exptl_absorpt_correction_type' value 'Gaussian' changed to
'gaussian' according to
/home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 

The following automatic conversions were performed:

'_refine_ls_weighting_scheme' value 'calc
w=1/[\s^2^(Fo^2^)+(0.0263P)^2^+1.0582P] where P=(Fo^2^+2Fc^2^)/3' was
changed to 'calc'. New tag '_refine_ls_weighting_details' was
created. The value of the new tag was set to
'w=1/[\s^2^(Fo^2^)+(0.0263P)^2^+1.0582P] where P=(Fo^2^+2Fc^2^)/3'.

Automatic conversion script
Id: cif_fix_values 3143 2015-03-26 13:38:13Z robertas 
;
_cod_original_sg_symbol_H-M      R-3m
_cod_original_formula_sum        'Cl4 H18 N6 O8 Rb1 Ru1'
_cod_database_code               2003156